Unusual Dewetting of Thin Polymer Films in Liquid Media Containing a Poor Solvent and a Nonsolvent Lin Xu,† Ashutosh Sharma,*,‡ Sang Woo Joo,† Hui Liu,§,∥ and Tongfei Shi*,§ †
School of Mechanical Engineering, Yeungnam University, Gyongsan 712-749, South Korea Department of Chemical Engineering, Indian Institute of Technology, Kanpur 208016, India § State Key Laboratory of Polymer Physics and Chemistry, Changchun Institute of Applied Chemistry, Chinese Academy of Sciences, Changchun 130022, P. R. China ∥ Department of Physics, Jilin University, Changchun 130012, P. R. China ‡
ABSTRACT: We investigate the control of pattern size and kinetics in spontaneous dewetting of thin polymer ﬁlms (polystyrene) that are stable to thermal annealing by annealing in a poor solvent (acetone)/nonsolvent (ethanol or n-hexane) liquid mixture. Dewetting occurs by the formation and growth of circular holes that coalesce to form droplets. The inﬂuence of the nature and the volume fraction of the nonsolvents on the contact angle of polymer droplets, number density of holes, and the kinetics of holes formation and growth is studied. Addition of ethanol greatly increases the hole density and slows down the kinetics substantially, while aﬀecting only a small change in wettability. n-Hexane addition shows an interesting nonmonotonic response in decreasing the hole density and contact angle in the volume fraction range of 0−0.3 but an opposite eﬀect beyond that. Although the two nonsolvents chosen cannot by themselves induce dewetting, their relative aﬃnity for the solid substrate vis-à-vis acetone can strongly inﬂuence the observed dewetting scenarios that are not understood by the existing theoretical considerations. n-Hexane, for example, has great aﬃnity for silicon substrate. In addition to the changes in wettability, viscosity, and ﬁlm interfacial tension engendered by the nonsolvents, the possibility of the formation of adsorbed liquid layers at the substrate−polymer interface, which can modify the interfacial friction and slippage, needs to be considered.
Dewetting of thin ﬁlms is a good model system for investigating the low dimensional physics of polymer chains in a melt, but most of dewetting studies have been by thermal annealing above the glass transition. Gabriele and co-workers21,22 showed the transition from the elasticity-dominated regime to a viscosity-dominated regime via the dewetting kinetics of holes growth and the shape of the rim. Recently, Tsui’s research group23−25 reported the change of the glass transition temperature of polymer chains with the ﬁlm thickness by a thermal dewetting process. Another route to trigger thin ﬁlm dewetting is by exposure to the vapors of a good solvent, which reduces the glass transition temperature below room temperature.26−30 The solvent-vapor-induced dewetting largely parallels the characteristics of the thermal dewetting in that the stabilizing surface tension is largely unaltered and thus the length scale of the surface instability cannot be varied except by a change in the ﬁlm thickness and by relaxation of residual stresses in the high molecular weight ﬁlms.26,27 Thus, control and miniaturization of the instability
INTRODUCTION Spontaneous instability and dewetting of ultrathin ( acetone > ethanol. n-Hexane completely spread on the substrate. Another indicator of the aﬃnity of a liquid for a substrate in air is the energy of adhesion, ΔG1L = γ1L − γ1 − γL, which together with the Young’s equation γL cos θ + γ1L = γ1 gives ΔG1L = −γL(1 + cos θ). Here γij are interfacial tensions and the subscripts correspond to silicon substrate (1) and solvent (L); θ > 0 is the
γ23 cos θ + γ12 = γ13
where γij are interfacial tensions and the subscripts correspond to silicon substrate (1), polymer (2), and liquid mixture (3); θ is the contact angle. According to the Young’s equation: cos θpolymer on Si = (γsolvent/Si − γpolymer/Si)/γpolymer/solvent. As θpolymer on Si > 90°, cos θpolymer on Si is smaller than zero in the case of the mixed solvent between acetone and ethanol. When the nonsolvent (ethanol) fraction increases, both γpolymer/solvent and γsolvent/Si should increase somewhat. However, both of these changes should decrease the contact angle, θpolymer on Si, which is the opposite of our experimental results. Clearly, the situation is more complex as γpolymer/Si is not simply the interfacial tension of dry polymer but that in its saturated state with the solvents. Thus, γpolymer/Si should also increase by the addition of a nonsolvent (ethanol). This is aided by the shrinkage of polymer chains to form globules with enhanced interchain interaction36 but weakened interaction with the substrate. Further, with increased ethanol fraction, the Si−PS interface may also contain more of ethanol, thus increasing the interfacial energy of this composite interface. However, in comparison with the case of n-hexane 14812
dx.doi.org/10.1021/la503319w | Langmuir 2014, 30, 14808−14816
and a continued slow increase in the PS−mixed solvents interfacial tension together with a decrease in substrate− mixture interfacial tension can once again increase the contact angle somewhat. Clearly, understanding of the contact angle decrease by n-hexane addition requires a modiﬁcation of the PS−substrate interface in a profound way. The contact angle discussed above reﬂects the wetting propensity of dewetted PS drops on silicon wafer in the presence of surrounding liquid mix as the droplets freeze in that position upon removal from the liquid. When these droplets were heated in air, their contact angle decreased slowly with time (for example, the droplets of initial contact angle of about 120° obtained by acetone annealing respread to ∼30° angle after 12 h of annealing at 180 °C). This is again expected on oxide-denuded silicon, on which the PS ﬁlm is stable under thermal annealing. This observation clearly indicates the role of acetone and other liquids in producing a large three-phase contact angle leading to dewetting. However, the kinetics of spreading was slow, which is likely due to the modiﬁcation of reactive silicon surface by adsorption of PS chains (autophobicity)13 and growth of even a monolayer of oxide. Both of these factors can change the short-range interactions at the contact profoundly and could produce nonzero, but small, equilibrium contact angles.13,39,46 In what follows, we examine the number density of holes and the kinetics of dewetting in view of the discussion above. As a cautionary note before proceeding further, we note that the experimental results presented, as novel and interesting as they are, are in conﬂict with our existing theoretical understanding on several counts that we discuss candidly below with an eﬀort to suggest new insights and to stimulate further work on the complex physics of four component (substrate−ﬁlm−solvent− nonsolvent) unstable thin polymer ﬁlms. We ﬁrst note that the maximum number density of holes, N, in a thin ﬁlm is governed by a competition between the destabilizing intersurface interactions and stabilizing interfacial tensions (thermodynamic factors) rather than the kinetic or transport factors (viscosity).6,14,19,38,39,46
discussed below, which has good aﬃnity for the Si interface, ethanol accumulation at this interface should be minimal and the small changes in the contact angle seem to be of entropic origin. The case of n-hexane addition is rather more curious (Figure 9b) in that the contact angle decreases sharply from around 120° in pure acetone to around 30° at an n-hexane volume fraction of 0.3 and then recovers slowly to around 60° at an nhexane volume fraction of 0.7. In the ﬁrst stage or regime of low n-hexane fraction, PS−mixed solvents interfacial tension (and thus contact angle) should increase with the addition of a nonsolvent. Thus, this ﬁnding indicates a concurrent reduction in the PS−substrate (silicon wafer) interfacial tension and a possible increase in the substrate−solvent interfacial tension that dominates over the increase in the PS−mixed solvents interfacial tension below a moderate volume fraction of nhexane (0−0.3). The contact angles of pure acetone and pure n-hexane on PS ﬁlm were measured to be 12° and 10° (error 1°), respectively. According to the Young’s equation γpolymer/solvent = γpolymer/air − γsolvent/air cos θsolvent on polymer film
Thus, γpolymer/solvent should increase by a few mN/m with the increase of the volume fraction of n-hexane to 0.3 because the surface tension of n-hexane is smaller than that of acetone by about 5 mN/m and the contact angle θsolvent on polymer film is rather invariant with the adding of n-hexane. The use of eq 2 for a drop of acetone/n-hexane mixture on polystyrene would thus show that only a small monotonic increase of γ23 cannot explain the great change of the equilibrium contact angles of the dewetted PS droplets from 117° to around 30°, when only 30% volume fraction n-hexane is added into mixture with a change in the value of cos θ from negative to positive. Clearly, the mixture composition is aﬀecting the PS−substrate (γ12) and substrate−mixture (γ13) interfacial tensions rather more profoundly, which can explain the variation of the contact angle as announced. According to eq 2, (γ13 − γ12) must change from negative to positive in the ﬁrst stage. The ﬁrst possible reason is that γ13 (γsolvent/Si) rapidly increases with the adding of n-hexane. According to Young’s equation, γsolvent/Si = γSi/air − γsolvent/air cos θsolvents on Si, γ13(γsolvent/Si) indeed increases with the adding of n-hexane because the surface tension of n-hexane is smaller. However, this is not suﬃcient to explain the contact angle variation from 117° to around 30°, when only 30% volume fraction n-hexane is added into mixture. The second possible reason is that the Si−polymer interfacial tension (γ12) greatly decreases with the adding of n-hexane. Enrichment/ adsorption of n-hexane at the substrate−polymer interface owing to its strong aﬃnity for the substrate (Figure 9c) could sharply decrease γ12, thus decreasing the contact angle, as observed. In addition, this view also successfully explains the kinetics of holes growth with a sharp decrease in the interfacial friction as discussed later. Thus, some increase of γsolvent/Si and, more importantly, the sharp decrease of γpolymer/Si are the factors that explain a sharp decline in the contact angle in the range of small n-hexane fraction. At larger fraction (>0.3), a small increase in the contact angle is similar to the increase seen in the case of ethanol and can be explained by small increases in the polymer−solvent and polymer−substrate interfacial tensions by the entropic eﬀects of the nonsolvent on the polymer chains. Thus, the aﬃnity of the nonsolvent for the substrate can strongly inﬂuence the contact angles of the dewetted PS droplets. As the n-hexane volume fraction becomes larger (>0.3), the substrate adsorption induced eﬀects should saturate
N = λ−2 ∼ [−(∂ 2ΔG /∂h2)/γ23]
where λ is the dominant length scale of the instability or the mean distance between the holes, ΔG is the excess energy of the intersurface interactions per unit area, γ23 is the PS− solution interfacial tension, and h is the ﬁlm thickness. A negative value of the spinodal parameter [−(∂2ΔG/∂h2)] indicates spontaneous dewetting by ampliﬁcation of surface instability. We had earlier shown that owing to closely matched van der Waals properties of PS and organic solutions, the net apolar van der Waals force in such systems is negligible or even slightly stabilizing.33 The genesis of thin ﬁlm stability is thus traced to the polar interactions induced by the presence of acetone.6,33 It has been shown that the excess thin ﬁlm energy (and spinodal parameter) can be related to the macroscopic parameters of wetting, −(∂2ΔG/∂h2) ∼ γ23 f(θ),6,39 where f(θ) is an increasing function of θ, so that N increases with the contact angle, θ. While quantitative evaluations are not possible because there is no direct method to quantify the apolar and polar interactions in this complex multiphase system with likely interfacial segregation of some components, the qualitative picture is fairly clear. The fact that a stronger instability or greater density of holes should result on a more nonwettable substrate (higher θ) is physically understandable, and indeed, 14813
dx.doi.org/10.1021/la503319w | Langmuir 2014, 30, 14808−14816
limitation reﬂected in an increased viscosity aided maybe by a decrease in slippage, as discussed above. Both of these favor a reduction in the dewetting velocity. Adding of nonsolvents should decrease the mobility of PS chains owing to their increasing collapse with increased nonsolvent concentration. This factor could overwhelm the eﬀect of changes brought about by a slight increase in the contact angle with an increased volume fraction of ethanol. A slowdown in the kinetics of holes formation and their subsequent growth also allows an opportunity for the growth of new holes in the areas which have not yet dewetted. This explains a greater propensity for a continued appearance of new holes with a nonsolvent (Figure 8) compared to acetone alone where all the holes appear rapidly in the initial phase and the hole-density remains nearly constant thereafter until the onset of coalescence. These scenarios of a near simultaneous or continuous formation of holes are also seen in the van der Waals destabilized thermally annealed ﬁlms,12,39 but the inﬂuence of polar interactions in this process is not yet addressed. Similarly, in the case of n-hexane as the nonsolvent, the variation of contact angle and the kinetics of hole growth are out-of-phase from theory. For example, the contact angle ﬁrst decreases and then increase with the increase in the volume fraction of n-hexane, implying (without considering the change of the viscosity of the ﬁlm) that the velocity of hole growth should ﬁrst decrease and then increase. However, interestingly, the experimental results are opposite to this argument. In the ﬁrst volume fraction regime (0−0.3), hole growth and hole formation become considerably faster, despite a substantial reduction in the contact angle and a putative increase in the viscosity owing to the presence of a nonsolvent! One should thus consider the interfacial segregation of hexane to play a profound role in this regime in greatly diminishing the friction and dissipation at the substrate, which is the rate-limiting factor determining the kinetics. As shown in Figure 9c, n-hexane indeed has a greater aﬃnity for the substrate, as indicated by its complete spreading, which should allow slippage of the polymer chains. As discussed before, the decrease in the contact angle of the PS droplets in this regime also indicates the formation of an ultrathin n-hexane layer or enriched zone at the substrate surface. The presence of a low-viscosity interlayer replacing the high viscosity adhering polymer chains can greatly decrease the viscous friction and thus enhance the kinetics. With further increase in the volume fraction beyond 0.3, the eﬀect of reduction in the interfacial friction reaches its limit, but the eﬀect of increasing ﬁlm viscosity with increased n-hexane content should now slow down the kinetics. In order to get further insight into the possible modiﬁcation of the substrate by n-hexane, we performed an additional experiment. In all of the experiments reported above, PS ﬁlms were immersed directly in a preprepared acetone/n-hexane mixture. Now, a PS ﬁlm was ﬁrst placed in pure liquid n-hexane for a long time (90 min), allowing slow diﬀusion through the ﬁlm but without any dewetting observed. Acetone was then rapidly added to hexane to form a mixture containing 5% volume fraction of hexane. The PS ﬁlms dewetted in such a mixture, as expected. However, dewetting was faster in the ﬁlm pre-equilibrated with hexane compared to the ﬁlm that was directly placed in the mixture (Figure 10). This observation also indicates a greater modiﬁcation of the substrate by nhexane, which allows a faster kinetics once acetone is added. We conclude by noting that the current understanding of thin polymer ﬁlm dewetting is limited to pseudo-single-phase
there should be no dewetting or holes when the substrate is completely wettable. The density of holes in Figures 3 (for ethanol) and 6 (for n-hexane) indeed generally mirror the variation of contact angles for the respective nonsolvents, as shown in Figure 9a,b. However, in the case of ethanol, this explanation of the change in hole density by a factor of 60 (inset of Figure 3) despite a relatively small change in wettability (117°−127° in Figure 9a) does not seem to be completely satisfactory and hints at involvement of other factors, such as nanophase separation and slippage at the substrate−polymer interface. As ethanol has much less aﬃnity compared to acetone for silicon substrate, it cannot form an enriched layer displacing acetone, but it could possibly reduce the enrichment of acetone there because of its solubility with ethanol. This factor may reduce the slippage of polymer chains induced by acetone enrichment with increased ethanol fraction. It is known that a decrease in the slippage (characterized by a slip length) increases the hole density.39,40 In contrast, addition of n-hexane should further increase slip owing to its greater aﬃnity for the substrate and thus reduce the hole density, in addition to the eﬀect on contact angle, as is evident until a volume fraction of 0.3. Beyond that, a saturation of the interface (slippage) should now make the hole density depend only on the contact angle. Understanding of the kinetics of hole formation and growth is even more complex compared to the thermodynamic arguments leading to the hole-density being governed by the contact angle or wettability. From a simple model of thin ﬁlm stability without considering any interfacial segregation or slip, the time scale for the appearance of holes is given by6,39 τ ∼ (μ /γ )[f (θ )]−2
where μ is the viscosity of the solvent-laden PS ﬁlm and f(θ) is an increasing function of θ as announced before. Further, the velocity, V, of hole growth (inverse of the time scale for hole growth)39,41−45 is given by V ∼ (γ /μ)[F(θ )]
where F(θ) is an increasing function of θ, which scales as θ in the limit of very small contact angles (Tanner’s law). Both eqs 4 and 5 are physically sound in that they predict that the time scales of hole formation and growth should increase on a more wettable substrate (smaller contact angle) as the instability becomes weaker. However, the experimental kinetic results in Figures 4, 7 (velocity of contact line retraction in ethanol and n-hexane), and 8 (time scales for the appearance or formation of holes) show an opposite trend than the theory predictions related to the inﬂuence of contact angle! For example, addition of ethanol increases the contact angle and should thus decrease the time for the formation of holes and increase the contact-line velocity, but the observations are just the opposite. The case of n-hexane is even more striking, where a nonmonotonic larger variation of the contact angle is observed, but the experimental results on the kinetics are again counterintuitive to the theory in that one sees an increase in the time scales or a slowing down with an increase in the contact angle and vice versa. Clearly, the other factors that aﬀect kinetics, such as the viscosity, interfacial tension, and the role of nonsolvent interfacial segregation,33 need to be considered. As argued before, interfacial segregation of ethanol at the substrate−ﬁlm boundary is not likely because of a much lower aﬃnity of ethanol for the silicon wafer as compared to acetone (Figure 9c). Thus, the major kinetic factor is the transport 3
dx.doi.org/10.1021/la503319w | Langmuir 2014, 30, 14808−14816
customary properties like the polymer chain mobility (viscosity), ﬁlm interfacial tension, and wettability (contact angle). Comparison with the existing theoretical ideas is more in the spirit of pointing out the gaps to motivate further work in the control of polymer thin ﬁlm equilibrium and dynamics by annealing under liquid mixtures. We suggest that the greater aﬃnity of a component to the substrate plays an important role in the formation of an ultrathin nanophase separated zone at the substrate−polymer interface that modiﬁes the contact angle and viscous friction and dissipation. Thus, unlike thermal or solvent-vapor-induced dewetting, room temperature dewetting under the liquid mixtures oﬀers a far greater control of the dewetting kinetics, shape of ﬁnal droplets (contact angle), and pattern dimensions, even in the stable ﬁlms.
*A.S. e-mail: [email protected]
*T.S. e-mail: [email protected]
Figure 10. OM images of the morphology of PS ﬁlms (67 ± 2 nm) placed either in a 5% n-hexane/acetone mixture (images a1 and a2) or pre-equilibrated in n-hexane for 90 min before addition of acetone to make a 5% n-hexane mixture (images b1 and b2). Morphologies in images a1 and b1 are at 20 s in the mixture and those of images a2 and b2 are at 60 s. The size of images are 300 × 225 μm2.
The authors declare no competing ﬁnancial interest.
ACKNOWLEDGMENTS This work is supported by the World Class University Grant No. R32-2008-000-20082-0 of the National Research Foundation of Korea, the National Natural Science Foundation of China (No. 21234007), and the Department of Science and Technology, India.
ﬁlms (melts) without considerations of very real polar interactions and interfacial segregation of liquid solvents/ nonsolvents that may occur owing to their diﬀering aﬃnities to the substrate. The novel experimental results presented here point to the diﬃculties in reconciling the observations with simple theories without taking into account additional dimensions. In any case, it is clear that the spontaneous dewetting of a thin polymer ﬁlm in mixed liquid solvents allows much greater control of the length and time scales compared to the widespread thermal and vapor phase annealing practices that exist.
(1) Yoneda, H.; Nishimura, Y.; Doi, Y.; Fukuda, M.; Kohno, M. Development of Microporous PE Films To Improve Lithium Ion Batteries. Polym. J. 2010, 42, 425−437. (2) Wang, X.; Yakovlev, S.; Beers, K. M.; Park, M. J.; Mullin, S. A.; Downing, K. H.; Balsara, N. N. On the Origin of Slow Changes in Ionic Conductivity of Model Block Copolymer Electrolyte Membranes in Contact with Humid Air. Macromolecules 2010, 43, 5306−5314. (3) Sandstrom, A.; Matyba, P.; Inganas, O.; Edman, L. Separating Ion and Electron Transport: The Bilayer Light-Emitting Electrochemical Cell. J. Am. Chem. Soc. 2010, 132, 6646−6647. (4) Siegel, A. P.; Murcia, M. J.; Johnson, M.; Reif, M.; Jordan, R.; Ruhe, J.; Naumann, C. A. Compartmentalizing a Lipid Bilayer by Tuning Lateral Stress in a Physisorbed Polymer-Tethered Membrane. Soft Matter 2010, 6, 2723−2732. (5) Huang, J. H.; Li, K. C.; Kekuda, D.; Padhy, H. H.; Lin, H. C.; Ho, K. C.; Chu, C. W. Efficient Bilayer Polymer Solar Cells Possessing Planar Mixed-Heterojunction Structures. J. Mater. Chem. 2010, 20, 3295−3300. (6) Sharma, A. Relationship of Thin Film Stability and Morphology to Macroscopic Parameters of Wetting in the Apolar and Polar Systems. Langmuir 1993, 9, 861−869. (7) Bandyopadhyay, D.; Sharma, A. Self-Organized Microstructures in Thin Bilayers on Chemically Patterned Substrates. J. Phys. Chem. C 2010, 114, 2237−2247. (8) Lim, S. K.; Perrier, S.; Neto, C. Patterned Chemisorption of Proteins by Thin Polymer Film Dewetting. Soft Matter 2013, 9, 2598− 2602. (9) Akhrass, S. A.; Reiter, G.; Hou, S. Y.; Yang, M. H.; Chang, Y. L.; Chang, F. C.; Wang, C. F.; Yang, A. C-M. Viscoelastic Thin Polymer Films under Transient Residual Stresses: Two-Stage Dewetting on Soft Substrates. Phys. Rev. Lett. 2008, 100, 178301. (10) Besancon, B. M.; Green, P. F. Dewetting Dynamics in Miscible Polymer−Polymer Thin Film Mixtures. J. Chem. Phys. 2007, 126, 224903.
CONCLUSIONS We have investigated the equilibrium and dynamic aspects of spontaneous room-temperature dewetting of thin polymer ﬁlms annealed under several liquid mixtures of a poor solvent (acetone) and a nonsolvent. Dewetting is characterized by the number density of holes (length scale) and the kinetics of hole formation and growth. The polystyrene ﬁlms on the oxide stripped silicon wafers considered are stable in air and resistant to dewetting by thermal annealing. Their dewetting under the solvent mixture (acetone/ethanol or acetone/n-hexane) proceeds by the introduction of polar interactions. The nature of the nonsolvent, its aﬃnity with the substrate vis-à-vis the solvent and its volume fraction all govern the polymer equilibrium wettability, hole density, and the kinetic aspects, which are often nonintuitive and theoretically not well understood. For example, addition of a 0.2 volume fraction of ethanol (nonsolvent) increases the hole density by a factor of 20 while simultaneously slowing the kinetic processes by several orders despite a very small change in the wettability. This ﬁnding oﬀers a general route to miniaturization of thin ﬁlm dewetting patterns. Nonmonotonic changes in the hole density and kinetics are witnessed with increased n-hexane content that are again out-of-phase with each other, the hole density being in-phase with the contact angle and the kinetics being out-ofphase with the contact angle variation. An explanation of these observations requires considering the factors beyond the 14815
dx.doi.org/10.1021/la503319w | Langmuir 2014, 30, 14808−14816
(11) Karapanagiotis, I.; Gerberich, W. W. Polymer Film Rupturing in Comparison with Leveling and Dewetting. Surf. Sci. 2005, 594, 192− 202. (12) Becker, J.; Grün, G.; Seemann, R.; Mantz, H.; Jacobs, K.; Mecke, K.; Blossey, A. Complex Dewetting Scenarios Captured by Thin-Film Models. Nat. Mater. 2003, 2, 59−63. (13) Reiter, G.; Khanna, R. Kinetics of Autophobic Dewetting of Polymer Films. Langmuir 2000, 16, 6351−6357. (14) Sharma, A.; Khanna, R. Pattern Formation in Unstable Liquid Films. Phys. Rev. Lett. 1998, 81, 3463−3466. (15) Reiter, G. Dewetting of Thin Polymer Films. Phys. Rev. Lett. 1992, 68, 75−78. (16) Reiter, G.; Akhrass, S. A.; Hamieh, M.; Damman, P.; Gabriele, S.; Vilmin, T.; Raphaël, E. Dewetting as an Investigative Tool for Studying Properties of Thin Polymer Films. Eur. Phys. J. Spec. Top. 2009, 166, 165−172. (17) Volodin, P.; Kondyurin, A. Dewetting of Thin Polymer Film on Rough Substrate: II. Experiment. J. Phys. D: Appl. Phys. 2008, 41, 065307. (18) Xu, L.; Sharma, A.; Joo, S. W. Instability and Pattern Formation Induced in Thin Crystalline Layers of a Conducting Polymer P3HT by Unstable Carrier Films of an Insulating Polymer. J. Phys. Chem. C 2012, 116, 21615−21621. (19) Xie, R.; Karim, A.; Douglas, J. F.; Han, C. C.; Weiss, R. A. Spinodal Dewetting of Thin Polymer Films. Phys. Rev. Lett. 1998, 81, 1251−1254. (20) Meredith, J. C.; Smith, A. P.; Karim, A.; Amis, E. J. Combinatorial Materials Science for Polymer Thin-Film Dewetting. Macromolecules 2000, 33, 9747−9756. (21) Gabriele, S.; Sclavons, S.; Reiter, G.; Damman, P. Disentanglement Time of Polymers Determines the Onset of Rim Instabilities in Dewetting. Phys. Rev. Lett. 2006, 96, 156105. (22) Gabriele, S.; Damman, P.; Sclavons, S.; Desprez, S.; Coppée, S.; Reiter, G.; Hamieh, M.; Akhrass, S. A.; Vilmin, T.; Raphaël, E. Viscoelastic Dewetting of Constrained Polymer Thin Films. J. Polym. Sci., Polym. Phys. 2006, 44, 3022−3030. (23) Yang, Z. H.; Fujii, Y.; Lee, F. K.; Lam, C.-H.; Tsui, O. K. C. Glass Transition Dynamics and Surface Layer Mobility in Unentangled Polystyrene Films. Science 2010, 328, 1676−1679. (24) Clough, A.; Peng, D. D.; Yang, Z. H.; Tsui, O. K. C. Glass Transition Temperature of Polymer Films That Slip. Macromolecules 2011, 44, 1649−1653. (25) Yang, Z. H.; Clough, A.; Lam, C.-H.; Tsui, O. K. C. Glass Transition Dynamics and Surface Mobility of Entangled Polystyrene Films at Equilibrium. Macromolecules 2011, 44, 8294−8300. (26) Lee, S. H.; Yoo, P. J.; Kwon, S. J.; Lee, H. H. Solvent-Driven Dewetting and Rim Instability. J. Chem. Phys. 2004, 121, 4346−4351. (27) Xu, L.; Shi, T. F.; An, L. J. The Dewetting Dynamics of The Polymer Thin Film by Solvent Annealing. J. Chem. Phys. 2008, 129, 044904. (28) Fondecave, R.; Brochard-Wyart, F. Polymers as Dewetting Agents. Macromolecules 1998, 31, 9305−9315. (29) Kim, H. I.; Mate, C. M.; Hannibal, K. A.; Perry, S. S. How Disjoining Pressure Drives The Dewetting of a Polymer Film on a Silicon Surface. Phys. Rev. Lett. 1999, 82, 3496−3499. (30) Bormashenko, E.; Pogreb, R.; Musin, A.; Stanevsky, O.; Bormashenko, Y.; Whyman, G.; Barkay, Z. Patterning in Rapidly Evaporated Polymer Solutions: Formation of Annular Structures under Evaporation of the Poor Solvent. J. Colloid Interface Sci. 2006, 300, 293−297. (31) Verma, A.; Sharma, A. Enhanced Self-Organized Dewetting of Ultrathin Polymer Films under Water−Organic Solutions: Fabrication of Sub-Micrometer Spherical Lens Arrays. Adv. Mater. 2010, 22, 5306−5309. (32) Verma, A.; Sharma, A. Sub-40 nm Polymer Dot Arrays by SelfOrganized Dewetting of Electron Beam Treated Ultrathin Polymer Films. RSC Adv. 2012, 2, 2247−2249.
(33) Xu, L.; Sharma, A.; Joo, S. W. Dewetting of Stable Thin Polymer Films Induced by a Poor Solvent: Role of Polar Interactions. Macromolecules 2012, 45, 6628−6633. (34) Siretanu, I.; Chapel, J. P.; Drummond, C. Water−Ions Induced Nanostructuration of Hydrophobic Polymer Surfaces. ACS Nano 2011, 5, 2939−2947. (35) Siretanu, I.; Chapel, J. P.; Drummond, C. Substrate Remote Control of Polymer Film Surface Mobility. Macromolecules 2012, 45, 1001−1005. (36) Rubinstein, M.; Colby, R. H. Polymer Physics; Oxford University Press: Oxford, UK, 2003; pp 144, 174. (37) Reiter, G. Unstable Thin Polymer Films: Rupture and Dewetting Processes. Langmuir 1993, 9, 1344−1351. (38) Reiter, G.; Khanna, R.; Sharma, A. Enhanced Instability in Thin Liquid Films by Improved Compatibility. Phys. Rev. Lett. 2000, 85, 1432−1435. (39) Sharma, A. Many Paths to Dewetting of Thin Films: Anatomy and Physiology of Surface Instability. Eur. Phys. J. E 2003, 12, 397− 408. (40) Kajari, K.; Sharma, A.; Khanna, R. Instability, Dynamics, and Morphology of Thin Slipping Films. Langmuir 2004, 20, 244−253. (41) Brochard-Wyart, F.; de Gennes, P. G.; Hervert, H.; Redon, C. Wetting and Slippage of Polymer Melts on Semi-Ideal Surfaces. Langmuir 1994, 10, 1566−1572. (42) Brochard-Wyart, F.; Debrégeas, G.; Fondecave, R.; Martin, P. Dewetting of Supported Viscoelastic Polymer Films: Birth of Rims. Macromolecules 1997, 30, 1211−1213. (43) Brochard-Wyart, F.; Daillant, J. Drying of Solids Wetted by Thin Liquid Films. Can. J. Phys. 1990, 68, 1084−1088. (44) Jacobs, K.; Seemann, R.; Schatz, G.; Herminghaus, S. Growth of Holes in Liquid Films with Partial Slippage. Langmuir 1998, 14, 4961− 4963. (45) Seemann, R.; Herminghaus, S.; Neto, C.; Schlagowski, S.; Podzimek, D.; Konrad, R.; Hubert Mantz, H.; Jacobs, K. Dynamics and Structure Formation in Thin Polymer Melt Films. J. Phys.: Condens. Matter. 2005, 17, S267−S290. (46) Seemann, R.; Herminghaus, S.; Jacobs, K. Dewetting Patterns and Molecular Forces: A Reconciliation. Phys. Rev. Lett. 2001, 86, 5534−5537. (47) Sherrington, D. C. Preparation, Structure and Morphology of Polymer Supports. Chem. Commun. 1998, 21, 2275−2286. (48) Sadek, P. The HPLC Solvent Guide; Wiley-Interscience Press: New York, 2002; p 23.
dx.doi.org/10.1021/la503319w | Langmuir 2014, 30, 14808−14816